## Evidence of electron interaction with an unidentified bosonic mode in superconductor CsCa2Fe4As4F2

Peng Li 1 , Sen Liao 1 , Zhicheng Wang 2 , Huaxun Li 3 , Shiwu Su 1 , Jiakang Zhang 1 , Ziyuan Chen 1 , Zhicheng Jiang 4,5 , Zhengtai Liu 6 , Lexian Yang 7 , Linwei Huai 8 , Junfeng He 8 , Shengtao Cui 4 , Zhe Sun 4 , Yajun Yan 1 , Guanghan Cao 3 , Dawei Shen 4,5 , Juan Jiang 1 † , Donglai Feng 1, 4,5,9 †

1 Shool of Emerging Technology, University of Science and Technology of China, Hefei 230026, China 2 Key Laboratory of Quantum Materials and Devices of Ministry of Education, School of Physics, Southeast University, Nanjing 211189, China

3 School of Physics, Zhejiang University, Hangzhou 310058, China

- 4 National Synchrotron Radiation Laboratory, University of Science and Technology of China, Hefei, 230026, China
- 5 School of Nuclear Science and Technology, University of Science and Technology of China, Hefei, 230026, China

6 Shanghai Synchrotron Radiation Facility, Shanghai Advanced Research Institute, Chinese Academy of Sciences, Shanghai 201210, China

7 State Key Laboratory of Low Dimensional Quantum Physics, Department of Physics, Tsinghua University, Beijing 100084, China

8 CAS Key Laboratory of Strongly-coupled Quantum Matter Physics, University of Science and Technology of China, Hefei, Anhui 230026, China

9 New Cornerstone Science Laboratory, University of Science and Technology of China, Hefei, 230026, China

Emails: jjiangcindy@ustc.edu.cn; dlfeng@ustc.edu.cn

## Abstract:

The kink structure in band dispersion usually refers to a certain electron-boson interaction, which is crucial in understanding the pairing in unconventional superconductors.  Here we report the evidence of the  observation  of  a  kink  structure  in  Fe-based  superconductor  CsCa2Fe4As4F2  using  angle-resolved photoemission spectroscopy. The kink shows an orbital selective and momentum dependent behavior, which is located at 15 meV below Fermi level along the Γ - Μ direction at the band with dxz orbital character and vanishes when approaching the Γ - Χ direction, correlated with a slight decrease of the superconducting gap. Most importantly, this kink structure disappears  when the superconducting gap closes, indicating that the corresponding bosonic mode  (~ 9 ± 1 meV)  is closely related to superconductivity. However, the origin of this mode remains unidentified, since it cannot be related to phonons or the spin resonance mode (~ 15 meV) observed by inelastic neutron scattering. The behavior of this mode is rather unique and challenges our present understanding of the superconducting paring mechanism of the bilayer FeAs-based superconductors.

## Introduction

Electron-boson  coupling  is  the  cornerstone  for  pairing  in  superconductors.  In  Bardeen-Cooper-

Schrieffer theory for conventional superconductors, phonons are identified as the pairing glue. While for unconventional superconductors, such as cuprates and Fe-based superconductors, antiferromagnetic

(AFM) magnons or spin excitations are often considered as the potential pairing bosonic mode. Particularly,  spin  resonance  mode  observed  by  inelastic  neutron  scattering  (INS)  correlates  with superconductivity. For example, it emerges below the superconducting transition temperature ( TC ), its energy ( ER ) correlates with TC and its momentum connects different parts of the Fermi surface [1-12] . The resonance  energy ER approximately  follows  an  empirical  ratio 𝐸𝑅/2Δ ~ 0.64 , where Δ is the superconducting gap  [3,13,14] . The observation of a smaller ER compared to 2Δ provides evidence for the existence of a spin exciton. On the other hand, numerous experiments reported the evidence of electronphonon coupling in these materials [15-25] , and other proposals of pairing glue such as orbital fluctuations [26-28] ,  add more complexity to the investigation of unconventional superconductivity.

Recently, a stochiometric Fe-based superconductor, ACa2Fe4As4F2 (A=K, Rb, Cs)  [29] , has attracted attention  due  to  their  multiple-layer  structures  and  a  high TC of  around  30  K.  However,  its  pairing symmetry remains controversial. Several muon-spin relaxation ( μsR ) measurements  [30-32] suggested the possible  nodal  superconducting  gaps,  while  other  methods  indicated  the  nodeless  gap  feature [33-38] . Interestingly, INS experiments reported resonance peaks with energies even higher than 2Δ which cannot be understood by the spin exciton picture [13,39] . This sets them apart from other Fe-based superconductors, and the presence of such atypical resonance peaks appears to challenge the AFM spin fluctuation scenario, sparking renewed interest in their pairing mechanisms.

In this Letter, we present a comprehensive angle-resolved photoemission spectroscopy (ARPES) investigation of the low-energy electronic structure of CsCa2Fe4As4F2 (TC~ 29 K). Our findings reveal a pronounced kink structure  that  is  strongly  correlated  with  superconductivity.  It  appears  at  a  binding energy ( EB ) of 15 meV along the Γ - Μ direction exclusively in the 𝛼 band ( dxz ), and disappears above the superconducting gap closing temperature. The kink exhibits strong angular dependent behavior, and diminishes  in  the Γ - Χ direction,  giving  a  dramatic  change  in  the  electron-boson  coupling  strength ( 𝜆𝑒-𝑏 ). Additionally, we observe that the anisotropic superconducting gap of the 𝛼 band closely follows the anisotropic behavior of this kink. Based on the size of the corresponding superconducting gap and kink energy, we propose a bosonic mode with an energy of around 9 meV which is highly related to superconductivity in this bilayer system. However, unlike the kink observed in Ba0.6K0.4Fe2As2 [40] , the kink in CsCa2Fe4As4F2 cannot be directly attributed to the reported spin resonance mode and its origin remains mysterious.

## Results and Discussion

The crystal structure of CsCa2Fe4As4F2, depicted in Fig. 1(a), can be regarded as a composite of CaFeAsF and KFe2As2. It exhibits a total doping level of 0.25 hole/Fe due to the self-doping effect [29] . Figures 1(b-d) show the basic electronic structure of the sample. The measured Fermi surface using 50 eV photons at 10 K is presented in Fig. 1(b). Around the Γ point, there are three hole pockets (   , and  ) while  four  hot  spot-like  pockets  (  ) surround  the Μ point,  more  details  could  be  found  in Supplementary Fig. 1 and Supplementary Fig. 2. One should notice that as a bilayer system, there should be two sets of Fe orbitals, and we neglect this in our discussion hereafter due to the fact that the interlayer coupling is weak in this system and the splitting of these bands is beyond our experimental resolution [35] .  The  quasi  two-dimensional  electronic  structure  of  this  compound  is  confirmed  by kz -dependent measurements in Supplementary Fig.3,  which is consistent with previous transport measurements where there was huge resistivity anisotropy of 𝜌𝑐 (𝑇)/𝜌 𝑎𝑏 (𝑇) up to 10 3 [41] . In addition to the primary bands, there exists a weak large pocket around the Μ point, as indicated by the white dashed curves. This is believed  to  be  the  folded 𝛾 band  from  the Γ point  (black  solid  circle)  due  to  surface  reconstruction, similar  to  other  alkali  metal  intercalated  Fe-based  superconductors [42,43] ,  indicating  most  likely  the measured samples are with Cs terminated surface. Both linear-horizontal (LH) and linear-vertical (LV) polarizations are utilized to detect the orbital characters of these bands, as shown in Figs. 1(b) and (c). The LV polarization exhibits a stronger intensity of the 𝛼 band, indicating its dxz orbital nature [44] .  The 𝛽 and 𝛾 bands around Γ are formed by dyz and dxy orbitals, respectively, while the 𝛿 and 𝜀 bands at the Μ point consist of dyz and dxy orbitals, respectively. Notably, a distinct kink structure is observed in the 𝛼 band well below TC as depicted in Fig. 1(e), located at 15 meV below the Fermi level. This kink anomaly is distinct from a Bogoliubov bending band since the energy positions differs (Supplementary Fig. 4) and it is also confirmed by our scanning tunneling microscopy (STM) result in Supplementary Fig. 5. More details about the kink will be discussed in the later.

Figure 2 displays the superconducting gaps and their angular dependence across different bands. The symmetrized spectra along the Γ - Μ direction measured at 7 K shown in Figs. 2(a) and 2(b) reveal a distinct gap opening at 𝛼 𝛽 , and 𝛿 bands. It should be noted that the  band may exhibit a tiny gap beyond energy resolution. The superconducting gap values ( Δ )  for the 𝛼 , 𝛽 and 𝛿 bands are 6 meV, 6 meV, and 5.5 meV, respectively [Fig. 2(c) and Supplementary Fig. 6], determined from the fitting of the symmetrized  energy  distribution  curves  (EDCs)  in  a  BCS-based  phenomenological  model [45] .  The temperature evolution of these bands can be found in  Supplementary Fig. 7. Figures 2(d)-(e) present momentum distributions of the symmetrized EDCs for the 𝛼 and  bands. The extracted gap values reveal a  slight  anisotropy  in  the 𝛼 band,  with  the  gap  size  gradually  decreasing  from  6  meV  in  the Γ - Μ direction to 4 meV in the Γ - Χ direction as shown in Fig. 2(f). However, the 𝛽 band is nearly isotropic, with a constant gap size of 6 meV as shown in Fig. 2(g). More details can be found in Supplementary Fig. 8.

The kink feature is exclusively observed at the 𝛼 band and strongly coupled with superconducting phase (Fig. 3). The criterion of the existence of kink is that both the real (Re  ) and imaginary part (Im  ) of the self-energy (  ) appear anomalies around the kink energy. When the superconducting gap closes, both the raw spectrum (the lower two panels of Fig. 3(a)) and the extracted peak positions (Fig. 3(d)) indicate an absence of this kink, where we use multiple Lorentzian peaks to present the fitted bands as shown in Supplementary Fig. 9. In the light of the extracted momentum distribution curves (MDCs) for the 𝛼 band at 7 K (Fig. 3(b)), we have identified the kink position located at 15 meV below EF highlighted by the blue curve, where there is a dramatic change in slope. The self-energy analysis of the 𝛼 band is shown in Fig. 3(c). Both the real and imaginary parts of the self-energy exhibit anomalies around this energy, and the Re  displays a relatively broad feature (ranging from 6 meV to 35 meV) with a maximum at 15 meV. Such a broad energy span is peculiar and intriguing (the data can be repeated on another sample  in  Supplementary  Fig.  10).  The  Kramers-Kronig  (KK)  transformation  analysis  is  shown  in Supplementary Fig. 11, which presents that both Re  and Im  match well with each other under the KK transformation, indicating the self-consistency of the extracted self-energies. The strength of electronboson coupling ( 𝜆𝑒-𝑏 )  of the kink can be determined by analyzing the slope change in both bare and renormalized band dispersions, where 𝜆𝑒-𝑏 is defined as:

$$\lambda _ { e - b } = \sqrt { ( \frac { d \varepsilon } { d k } ) } _ { b a r e } \Big / _ { ( \frac { d \varepsilon } { d k } ) } - 1$$

We use the curve at 100K as the bare band, and the energy range of the renormalized band lies between the gap energy and the kink energy. The extracted 𝜆𝑒-𝑏 values gradually decrease with the increasing temperature, and eventually disappears above the superconducting gap closing temperature, as shown in Fig. 3(e). Details of the kink structure evolution with temperature can be found in Supplementary Fig. 12-14. One could notice that the kink seems to persist slightly above the transition temperature 29 K and vanishes around 35 K, which is possible due to the existence of pseudogap in this material as reported by several other experiments [46,47] .

We further analyze the angular distribution of the kink in the 𝛼 band well below TC in Fig. 4. Figures. 4(a)  and  4(d)  depict  the  representative  high  symmetry  cuts  along  the Γ - Χ and Γ - Μ directions, respectively (more details can be found in Supplementary Fig. 15). The angle offset from the Γ - Μ direction is defined as 𝜃 . The kink structure is present along the Γ - Μ direction, while it is absent along the Γ - Χ direction. The self-energy analysis also reveals discernible distinctions between these two directions, as illustrated in Figs. 4(b) and 3(c). In contrast to the observable anomalous signals around 15 meV in the Γ - Μ direction,  no  significant  variation  is  observed  in  both  Re  and  Im  in  the Γ - Χ direction. The peak positions of the 𝛼 band are extracted step by step from the Γ - Μ direction to the Γ - Χ direction with a 5-degree increment, as summarized in Fig. 4(c) with momentum shifts. The dashed straight  lines  serve  as  guides  for  the  kink  positions  at  each  curve  and  the  determination  of  the  kink position is in Supplementary Fig. 16. Figure 4(e) shows that both the kink energy position 𝐸𝑘𝑖𝑛𝑘 and the corresponding  coupling  strength 𝜆𝑒-𝑏 exhibit  remarkable  decreasing  trends  as 𝜃 increases.  The  kink vanishes beyond 25 , accompanied by a slight energy shift from 15 meV at 0 ° ° to 13 meV at 25 .  Notably, ° the  coupling  strength  also  dramatically  decreases  towards  zero  at  the  edge  of  25 ° .  In  spectroscopic experiments, electron-boson interactions may give rise to low energy anomalies near the Fermi level, appearing at energies of ∆ + Ω in principle, where ∆ represents the superconducting gap and Ω denotes the corresponding bosonic energy. We extract the boson energies at various angles by subtracting the ∆𝛼 from 𝐸𝑘𝑖𝑛𝑘 .  As shown in Fig. 4(f), the extracted boson energies are located at a constant value of 9 ± 1 meV. Therefore, it is reasonable to infer that the distribution of the electron-boson coupling correlates with the anisotropic superconducting gap of the 𝛼 band  [48] .

A common origin of such a kink in band dispersion is electron-phonon coupling, which renormalizes the Fermi velocity around the phonon energy Ω [49] . For ACa2Fe4As4F2 (A=K, Rb, Cs), numerous phonon modes have been detected in various experiments  [34,46,50,51] , and these modes were observed in both the normal and superconducting phases. In our ARPES experiment, however, the absence of kink behavior above TC exclude phonon as a candidate. The 9 meV bosonic mode is directly associated with a mode that should only emerge when the superconducting condensation is ready, and several other experiments have also reported a potentially superconducting correlated bosonic mode in ACa2Fe4As4F2 [36,38,52] .

The spin resonance has been discovered to emerge in the superconducting states of cuprates and iron-based  superconductors [2,4,6,7,11,53-60] . While  the  correlation  between  kink  structures  and  the corresponding spin resonance modes have been widely reported in cuprates  [9,61-63] , in which these kinks are located at the energy 𝐸𝑘𝑖𝑛𝑘 = ∆ + 𝐸𝑅 [63] , only a few  Fe-based  superconductors,  such  as Ba0.6K0.4Fe2As2 [40] and (Sr/Ba)1-xKxFe2As2  [64] , were found to exhibit this correspondence. Notably, the kink discovered in CsCa2Fe4As4F2 which presents a broad distribution of Re  cannot be accounted for by the sharp spin resonance mode at 15 meV observed by the neutron scattering [13][39] , as the ARPES determined kink corresponds to a boson energy of 9 ± 1 meV . Therefore, we exclude the possibility of the reported spin resonance mode as being the physical origin of the kink. However, it is noteworthy that the Re  of the 𝛼 band presents a broad feature in energy where the spin resonance mode may exist within this broad spectrum, but with a limited impact.

These bilayer superconductors (ACa2Fe4As4F2) are quite unique among all iron-based superconductors.  On  one  hand,  it  shows  giant  anisotropy  between  the  in-plane  and  out-of-plane resistivity which is different from most iron pnictides and mimic cuprates 41 .  On the other hand, the spin resonance modes possess a unique downward dispersion that is similar to cuprates in previous INS report, and its energy exceeds the limit of 2∆ [13] , challenging the conventional understanding of the resonance modes. Due to the similarities to cuprates, one possible candidate for causing such a broad Re  in energy may be the existence of paramagnon, which is broad in energy and only observed in numerous cuprates by the resonant inelastic soft X-ray scattering but not by neutron scattering [65] . Another possible mode that emerges in superconducting state is Josephson plasmon, which only exists in the multiple-layered superconductors  [66-69] . Further optical measurements on thick samples are needed to study the Josephson plasmon.  If  true,  the  correlation  between  momentum  dependent  gap  and 𝜆𝑒-𝑏 may suggest  that  the electron-Josephson plasmon can further facilitate pairing in addition to other correlation effects. One could notice that, similar to spin resonance mode and electron-magnon coupling in multi orbital system [40,70] ,  this  mode  either  originated  from  paramagnon  or  Josephson  plasmon  also  has  a  strong  orbital selectivity here. Additionally, the extracted boson energy closely aligns with the spin gap energy (~ 10 meV) of this compound  [13] , suggesting that the spin gap might be also the possible candidate similar to the case in the overdoped Bi2Sr2CaCu2O8+δ  [71] . Considering that the strong superconductivity correlated kink  structures  are  rather  rare  in  other  iron-based  superconductors,  such  a  remarkable  kink  in  band dispersion is a unique feature observed for the bilayer system.

In conclusion, our ARPES study of CsCa2Fe4As4F2 presents a unique case that deviates from many other studied Fe-based superconductors. We reveal an anomalous kink in CsCa2Fe4As4F2 that exists just at the 𝛼 band, which is most likely caused by electron interacting with certain bosons. This kink exhibits strong  coupling  with  superconductivity  and  correlates  with  the  superconducting  gap  of  the 𝛼 band. However, it cannot be attributed to phonons and the spin resonance found by INS.  Our results may provide a counterexample that challenges the critical role of spin resonance in Fe-based superconductors. Finally, we believe that both the unique spin resonance mode in INS and the unique bosonic mode in our ARPES measurements can uncover some anomalous but critical aspects. The identity of this unique bosonic  mode  calls  for  further  study  which  could  be  crucial  to  understand  the  superconducting mechanism in Fe-based superconductors.

## Methods

High quality CsCa2Fe4As4F2 single crystals were synthesized by the solid-state reaction method [29,39] . Synchrotron-ARPES measurements were performed at beamline BL03U of Shanghai Synchrotron Radiation Facility (SSRF) and BL13U of National Synchrotron Radiation Laboratory (NSRL) in China . The overall energy resolution for the gap measurement was set to be better than 6 meV at 23 eV photon energy and the angular resolution is ~ 0.2 degree for the gap and kink measurements. The crystals were cleaved in-situ and measured with a base pressure better than 6 × 10 -11 Torr. Lab-based laser ARPES measurements were carried out using 6.999 eV light source at University of Science and Technology of China. The overall energy resolution was set to be better than 2 meV the angular resolution is ~ 0.2 degree for the gap and kink measurements. All the data presented in this paper were taken within a few hours after cleavage ensuring the results were not affected by aging effect.

## Data Availability

All data needed to evaluate the conclusion in the paper are present in the paper and the Supplementary information. All raw data generated during the current study are available from the corresponding author upon request.

## References

- 1 H. F. Fong, P. B., Y. Sidis, L. P. Regnault, A. Ivanov,G.D.Guk, N. Koshizuka &amp; B. Keimer. Neutron scattering from magnetic excitations in Bi2Sr2CaCu2O8. Nature 398, 588-591 (1999).
- 2 Christianson, A. D. et al. Unconventional superconductivity in Ba0.6K0.4Fe2As2 from inelastic neutron scattering. Nature 456 , 930-932 (2008).
- 3 Dai, P. Antiferromagnetic order and spin dynamics in iron-based superconductors. Reviews of Modern Physics 87 , 855-896 (2015).
- 4 Inosov,  D.  S. et  al.  Normal-state  spin  dynamics  and  temperature-dependent  spin-resonance energy in optimally doped BaFe1.85Co0.15As2. Nature Physics 6 , 178-181 (2009).
- 5 Lee,  C.  H. et  al.  Universality  of  the  dispersive  spin-resonance  mode  in  superconducting BaFe2As2. Phys. Rev. Lett. 111 , 167002 (2013).
- 6 Steffens, P. et al. Splitting of resonance excitations in nearly optimally doped Ba(Fe0.94Co0.06)2As2: an inelastic neutron scattering study with polarization analysis. Phys. Rev. Lett. 110 , 137001 (2013).
- 7 Xie,  T. et  al.  Odd  and  Even  Modes  of  Neutron  Spin  Resonance  in  the  Bilayer  Iron-Based Superconductor CaKFe4As4. Phys. Rev. Lett. 120 , 267003 (2018).
- 8 Capogna, L. et al. Odd and even magnetic resonant modes in highly overdoped Bi2Sr2CaCu2O8+δ. Physical Review B 75, 060502(R) (2007).
- 9 Eschrig,  M.  The  effect  of  collective  spin-1  excitations  on  electronic  spectra  in  high-Tc superconductors. Advances in Physics 55 , 47-183 (2007).
- 10 Tranquada, J. M., Xu, G. &amp; Zaliznyak, I. A. Superconductivity, antiferromagnetism, and neutron scattering. Journal of Magnetism and Magnetic Materials 350 , 148-160 (2014).
- 11 Wang,  Z. et  al.  Close  relationship  between  superconductivity  and  the  bosonic  mode  in Ba0.6K0.4Fe2As2 and Na(Fe0.975Co0.025)As. Nature Physics 9 , 42-48 (2012).
- 12 Liu, C. et al. Preferred Spin Excitations in the Bilayer Iron-Based Superconductor CaK(Fe0.96Ni0.04)4As4 with Spin-Vortex Crystal Order. Phys. Rev. Lett. 128 , 137003 (2022).
- 13 Hong, W. et al. Neutron Spin Resonance in a Quasi-Two-Dimensional Iron-Based Superconductor. Phys. Rev. Lett. 125 , 117002 (2020).
- 14 Shan,  L. et al. Evidence  of  a  spin  resonance  mode  in  the  iron-based  superconductor Ba0.6K0.4Fe2As2 from scanning tunneling spectroscopy. Phys. Rev. Lett. 108, 227002 (2012).
- 15 Yang, R. et al. Anomalous phonon behavior in superconducting CaKFe4As4: An optical study. Physical Review B 95 , 064506 (2017).
- 16 Zhuoyu Chen, Y. W., Slavko N. Rebec, Tao Jia, Makoto Hashimoto, Donghui Lu, Brian Moritz, Robert G. Moore, Thomas P. Devereaux, Zhi-Xun Shen. Anomalously strong near-neighbor attraction in doped 1D cuprate chains. Science 373, 1235-1239 (2021).
- 17 T. P. Devereaux, T. C., Z.-X. Shen, N. Nagaosa. Anisotropic Electron-Phonon Interaction in the Cuprates. Phys. Rev.  Lett. 93 , 117004 (2004).
- 18 C. Gadermaier, A. S. A., V. V. Kabanov, P. Kusar, T. Mertelj, X. Yao, C. Manzoni, D. Brida, G. Cerullo, and D. Mihailovic. Electron-Phonon Coupling in High-Temperature Cuprate Superconductors Determined from Electron Relaxation Rates. Phys. Rev. Lett. 105 , 257001(2010).

19

20

21

22

23

24

25

26

27

28

29

30

31

32

33

34

Seung Ryong Park, D. J. S., C. S. Leem, Chul Kim, C. Kim, B. J. Kim, and H. Eisaki. AngleResolved Photoemission Spectroscopy of Electron-Doped Cuprate Superconductors: Isotropic Electron-Phonon Coupling. Phys. Rev.  Lett. 101 , 117006 (2008). Fabian Schrodi, P. M. O., and Alex Aperis Unconventional superconductivity mediated solely by isotropic electron-phonon interaction. Phys. Rev. B 104 , L140506 (2021). C.W. Luo, * I. H. Wu, P. C. Cheng, J.-Y. Lin, K. H. Wu, T. M. Uen, J. Y. Juang, T. Kobayashi, D. A. Chareev, O. S. Volkova, and A. N. Vasiliev. Quasiparticle Dynamics and Phonon Softening in FeSe Superconductors. Phys. Rev.  Lett. 108 , 257006 (2012). L. Boeri, M. C., I. I. Mazin, O. V. Dolgov, and F. Mauri. Effects of magnetism and doping on the electron-phonon coupling in BaFe2As2. Phys. Rev. B 82 , 020506(R) (2010). Chaofan Zhang, Z. L., Zhuoyu Chen, Yanwu Xie, Ruihua He, Shujie Tang, Junfeng He, Wei Li, Tao Jia, Slavko N. Rebec, Eric Yue Ma, Hao Yan, Makoto Hashimoto, Donghui Lu, Sung-Kwan Mo, Yasuyuki  Hikita,  Robert  G.  Moore,  Harold  Y.  Hwang,  Dunghai  Lee  &amp;  Zhixun  Shen. Ubiquitous strong electron-phonon coupling at the interface of FeSe/SrTiO3. Nat. Commun. 8 , 14468 (2017). Huimin Zhang, D. Z., Xiaowei Lu, Chong Liu, Guanyu Zhou, Xucun Ma, Lili Wang, Peng Jiang, Qi-Kun Xue, &amp; Xinhe Bao. Origin of charge transfer and enhanced electron-phonon coupling in single unit-cell FeSe films on SrTiO3. Nat. Commun. 8 , 214 (2017). Yuanhe Song, Z. C., Qinghua Zhang, Haichao Xu, Xia Lou, Xiaoyang Chen, Xiaofeng Xu, Xuetao Zhu, Ran Tao, Tianlun Yu, Hao Ru, Yihua Wang, Tong Zhang, Jiandong Guo, Lin Gu , Yanwu Xie , Rui Peng &amp; Donglai Feng High temperature superconductivity at FeSe/LaFeO3 interface. Nat. Commun. 12 , 5926 (2021). Onari, S. &amp; Kontani, H. Self-consistent vertex correction analysis for iron-based superconductors: mechanism of Coulomb interaction-driven orbital fluctuations. Phys. Rev. Lett . 109 , 137001 (2012). Onari, S., Kontani, H. &amp; Sato, M. Structure of neutron-scattering peaks in both s++-wave and s±-wave states of an iron pnictide superconductor. Physical Review B 81 , 060504 (2010). Maier, T. A., Graser, S., Hirschfeld, P. J. &amp; Scalapino, D. J. Inelastic neutron and x-ray scattering as probes of the sign structure of the superconducting gap in iron pnictides. Physical Review B 83 , 220505 (2011). Wang, Z. C. et al. Superconductivity in KCa2Fe4As4F2 with Separate Double Fe2As2 Layers. J. Am. Chem. Soc. 138 , 7856-7859 (2016). Smidman, M. et al. Nodal multigap superconductivity in KCa2Fe4As4F2. Physical Review B 97 , 060509 (2018). Kirschner, F. K. K. et al. Two-gap superconductivity with line nodes in CsCa2Fe4As4F2. Physical Review B 97 , 060506 (2018). Devashibhai T. Adroja, F. K. K. K., Franz Lang, Michael Smidman, Adrian D. Hillier, ZhiCheng  Wang,  Guang-Han  Cao,  Gavin  B.  G.  Stenning,  and  Stephen  J.  Blundell.  Multigap Superconductivity in RbCa2Fe4As4F2 Investigated Using μSR Measurements. J. Phys. Soc. Jpn. 87 , 124705 (2018). Huang, Y. Y. et  al.  Multigap  nodeless  superconductivity  in  CsCa2Fe4As4F2  probed  by  heat transport. Physical Review B 99 , 020502 (2019). Xu, B. et al. Band-selective clean-limit and dirty-limit superconductivity with nodeless gaps in the bilayer iron-based superconductor CsCa2Fe4As4F2. Physical Review B 99 , 125119 (2019).

|   35 | Wu, D. et al. Spectroscopic evidence of bilayer splitting and strong interlayer pairing in the superconductor KCa 2 Fe 4 As 4 F 2 . Physical Review B 101 , 224508 (2020).                                                                                                                                                                                       |
|------|------------------------------------------------------------------------------------------------------------------------------------------------------------------------------------------------------------------------------------------------------------------------------------------------------------------------------------------------------------------|
|   36 | Duan, W. et al. Single-particle tunneling spectroscopy and superconducting gaps in the layered iron-based superconductor KCa 2 Fe 4 As 4 F 2 . Physical Review B 103 , 214518 (2021).                                                                                                                                                                            |
|   37 | Wang, T. et al. Low temperature specific heat of 12442-type KCa 2 Fe 4 As 4 F 2 single crystals. Science China Physics, Mechanics &Astronomy 63 , 297412 (2020).                                                                                                                                                                                                 |
|   38 | Torsello, D. et al. Nodal multigap superconductivity in the anisotropic iron-based compound RbCa 2 Fe 4 As 4 F 2 . npj Quantum Materials 7 , 10 (2022).                                                                                                                                                                                                          |
|   39 | Adroja, D. T. et al. Observation of a neutron spin resonance in the bilayered superconductor CsCa 2 Fe 4 As 4 F 2 . J. Phys. Condens. Matter 32 , 435603 (2020).                                                                                                                                                                                                 |
|   40 | Richard, P. et al. Angle-resolved photoemission spectroscopy of the Fe-Based Ba 0.6 K 0.4 Fe 2 As 2 high temperature superconductor: evidence for an orbital selective electron-mode coupling. Phys. Rev. Lett. 102 , 047003 (2009).                                                                                                                             |
|   41 | Wang, Z.-C. et al. Giant anisotropy in superconducting single crystals of CsCa 2 Fe 4 As 4 F 2 . Physical Review B 99 , 144501 (2019).                                                                                                                                                                                                                           |
|   42 | Xiong Yang, Z. D., Hai Lin, Delong Fang, Huan Yang, Xiyu Zhu, and Hai-Hu Wen. Vortex lattice and vortex bound states in CsFe 2 As 2 investigated by scanning tunneling microscopy/spectroscopy. Phys. Rev. B 98 , 024505 (2018).                                                                                                                                 |
|   43 | Delong Fang, X. S., Zengyi Du, Pierre Richard, Huan Yang, X. X. Wu, Peng Zhang, Tian Qian, Xiaxin Ding, Zhenyu Wang, T. K. Kim, M. Hoesch, Aifeng Wang, Xianhui Chen, Jiangping Hu, Hong Ding, and Hai-Hu Wen. Observation of a Van Hove singularity and implication for strong- coupling induced Cooper pairing in KFe 2 As 2 . Phys. Rev. B 92 , 144513(2015). |
|   44 | Zhang, Y. et al. Orbital characters of bands in the iron-based superconductor BaFe 1.85 Co 0.15 As 2 . Physical Review B 83 , 054510 (2011).                                                                                                                                                                                                                     |
|   45 | Matsui, H. et al. BCS-like Bogoliubov quasiparticles in high-T(c) superconductors observed by angle-resolved photoemission spectroscopy. Phys. Rev. Lett. 90 , 217002 (2003).                                                                                                                                                                                    |
|   46 | Ultrafast Optical Spectroscopy Evidence of Pseudogap and Electron-Phonon Coupling in an Iron-Based Superconductor KCa 2 Fe 4 As 4 F 2 . Science China Physics, Mechanics &Astronomy 65 237411 (2022).                                                                                                                                                            |
|   47 | Li, M. et al. Enhanced Nernst effect above Tc in the quasi-two-dimensional iron pnictide superconductor CsCa 2 Fe 4 As 4 F 2 . Physical Review B 105 , 104512 (2022).                                                                                                                                                                                            |
|   48 | Johnston, S. et al. Evidence for the Importance of Extended Coulomb Interactions and Forward Scattering in Cuprate Superconductors. Phys. Rev. Lett. 108 ,166404 (2012).                                                                                                                                                                                         |
|   49 | Borisenko, S. V. et al. One-Sign Order Parameter in Iron Based Superconductor. Symmetry 4 , 251-264 (2012).                                                                                                                                                                                                                                                      |
|   50 | Hao, J. et al. Pseudogap and strong pairing induced by incipient and shallow bands in quasi- two-dimensional KCa 2 Fe 4 As 4 F 2 . Physical Review B 106 , 014523 (2022).                                                                                                                                                                                        |
|   51 | Xu, B. et al. Superconductivity-induced transverse plasma mode and phonon anomaly in the c- axis response of the bilayer compound RbCa 2 Fe 4 As 4 F 2 . Physical Review B 101 , 214512 (2020).                                                                                                                                                                  |
|   52 | Piatti, E., Torsello, D., Ghigo, G. & Daghero, D. Spectroscopic studies of the superconducting gap in the 12442 family of iron-based compounds (Review article). Low Temperature Physics 49 , 770-785 (2023).                                                                                                                                                    |
|   53 | Korshunov, M. M. & Eremin, I. Theory of magnetic excitations in iron-based layered superconductors. Physical Review B 78 , 140509 (2008).                                                                                                                                                                                                                        |

54

55

56

57

58

59

60

61

62

63

64

65

66

67

68

69

Chi, S. et al. Inelastic neutron-scattering measurements of a three-dimensional spin resonance in the FeAs-based BaFe1.9Ni0.1As2 superconductor. Phys. Rev. Lett. 102 , 107006 (2009).

Lumsden, M. D. et al. Two-dimensional resonant magnetic excitation in BaFe1.84Co0.16As2. Phys. Rev. Lett . 102 , 107005 (2009).

- Qiu, Y. et al. Spin gap and resonance at the nesting wave vector in superconducting FeSe0.4Te0.6. Phys. Rev. Lett. 103 , 067008 (2009).
- Castellan,  J.  P. et  al.  Effect  of  Fermi  surface  nesting  on  resonant  spin  excitations  in  Ba(1x) KxFe2As2. Phys. Rev. Lett. 107 , 177003 (2011).
- Zhang, C. et al. Neutron scattering studies of spin excitations in hole-doped Ba0.67K0.33Fe2As2 superconductor. Sci. Rep. 1 , 115 (2011).
- Qureshi, N. et al. Anisotropy of incommensurate magnetic excitations in slightly overdoped Ba0.5K0.5Fe2As2probed by polarized inelastic neutron scattering experiments. Physical Review B 90 , 100502 (2014).
- Iida, K. et al. Spin  Resonance  in  the  New-Structure-Type  Iron-Based  Superconductor CaKFe4As4. Journal of the Physical Society of Japan 86 , 093703 (2017).
- A.  Kaminski,  M.  R.,  J.  C.  Campuzano,  M.  R.  Norman,  H.  Fretwell,  J.  Mesot,  T.  Sato,  T. Takahashi, and K. Kadowaki. Renormalization of Spectral Line Shape and Dispersion below Tc in Bi2Sr2CaCu2O8+δ. Phys. Rev.  Lett . 86 , 1070(2001).
- A. D. Gromko, A. V. F., Y.-D. Chuang, J. D. Koralek, Y. Aiura, Y. Yamaguchi, K. Oka, Yoichi Ando, and D. S. Dessau. Mass-renormalized electronic excitations at (π,0) in the superconducting state of Bi2Sr2CaCu2O8. Phys. Rev. B 68 , 174520(2003).
- Chubukov, A. A. a. A. V. A Relation between the Resonance Neutron Peak and ARPES Data in Cuprates. Phys. Rev. Lett. 83 , 1652 (1999).

Wray, L. et al. Momentum dependence of superconducting gap, strong-coupling dispersion kink, and  tightly  bound  Cooper  pairs  in  the  high-Tc(Sr,Ba)1-x(K,Na)xFe2As2  superconductors. Physical Review B 78, 184508 (2008).

M. Le Tacon, G. G., J. Chaloupka, M. Moretti Sala, V. Hinkov, M.W. Haverkort, M. Minola, M. Bakr, K. J. Zhou, S. Blanco-Canosa, C. Monney, Y. T. Song, G. L. Sun, C. T. Lin, G. M. De Luca, M. Salluzzo, G. Khaliullin, T. Schmitt, L. Braicovich and B. Keimer. Intense paramagnon excitations in a large family of high-temperature superconductors. Nature Physics 7 , 725-730 (2011).

Matsuda, Y., Gaifullin, M. B., Kumagai, K., Kadowaki, K. &amp; Mochiku, T. Collective Josephson plasma resonance in the vortex state of Bi2Sr2CaCu2O8+δ delta. Phys. Rev. Lett. 75 , 4512-4515 (1995).

- T.  Motohashi,  J.  S.,  K.  Kitazawa,  and  K.  Kishio,  K.  M.  Kojima  and  S.  Uchida,S.  Tajima. Observation  of  the  Josephson  plasma  reflectivity  edge  in  the  infrared  region  in  Bi-based superconducting cuprates. Phys. Rev. B 61 , R9269(R) (2000).
- Boris, A. V. et al. Josephson plasma resonance and phonon anomalies in trilayer Bi2Sr2Ca2Cu3O10. Phys. Rev. Lett. 89 , 277001 (2002).
- Singley, E. J. et al. Measuring the Josephson plasma resonance in Bi2Sr2CaCu2O8 using intense coherent THz synchrotron radiation. Physical Review B 69 , 092512 (2004)

70

Yu, T. L. et al. Strong band renormalization and emergent ferromagnetism induced by electronantiferromagnetic-magnon coupling. Nat. Commun. 13 , 6560 (2022).

- 71 Valla, T. Drozdov, I. K. and Gu, G. D. Disappearance of superconductivity due to vanishing

coupling in the overdoped Bi2Sr2CaCu2O8+δ. Nat. Commun . 11 , 569 (2020).

## Acknowledgements

This work is supported by the National Natural Science Foundation of China (Grant No. 12174362 and No. 11888101, No. 92065202), the Innovation Program for Quantum Science and Technology (Grant No. 2021ZD0302800, No. 2021ZD0302802), the New Cornerstone Science Foundation. Part of this research used Beamline 03U of the Shanghai Synchrotron Radiation Facility, which is supported by ME2 project under contract no. 11227902 from National Natural Science Foundation of China. The authors would like to express their gratitude for the insightful discussions with H. Q. Luo, X. Y . Lu. S. S. Qin, K. Jiang, and J. P. Hu.

## Author Contributions Statement

P. L. and J. J. conceived the experiments. P. L., S. L., S. W. S. and J.J. carried out ARPES measurements with the synchrotron assistance from Z. C. L., Z. T. L. and D. W. S. at SSRF, S. T. C. and Z. S. at NSRL and  laser-ARPES  assistance  from  L.  X. Y.,  L. W.  H.  and  J.  F.  H..  Z.  C. W,  H.  X.  Li  and  G.  H.  C. synthesized single crystals. J. K. Z., Z. Y . C. and Y . J. Y . conducted the STM experiments. P. L., J. J. and D. L. F. wrote the manuscript. All authors contributed to the scientific planning and discussions.

## Competing Interests Statement

The authors declare no competing interests.

## Figure Legends

FIG.  1. Basic  crystal  and  electronic  band  structure  of  CsCa2Fe4As4F2.  (a)  The  crystal  structure  of CsCa2Fe4As4F2. (b) and (c)  ARPES spectra along the Γ - Μ direction by using both LH and LV polarized 60 eV photons. The bands are denoted by α β γ δ , , , and ε .  (d) Fermi surface map obtained at 10 K using 50  eV  photons,  superposed  with  2Fe-Brillouin  zone  (BZ)  boundary  (yellow  solid  lines)  and  high symmetry points (black dots).  (e) Kink structure on the α band measured with 7 eV laser. The black arrow indicates the kink position and the black dashed line indicates the bare band in normal state.

![Image](https://ac.marcodsn.me/arxiv-markdown-images/2408.00469v1-figure-0e5b17dc-92cc-4ee8-a8c1-4143c6920f7e.jpg)

FIG. 2. Multiband superconducting gaps and their momentum distributions. (a) Symmetrized ARPES spectrum  along  the Γ - Μ direction  measured  at  7  K  with  23  eV  photons,  where 𝛼 , 𝛽 and 𝛾 denote distinct bands. The color bar shows the ARPES spectra intensity. (b) Symmetrized ARPES spectrum of the δ band measured near the M point along the Γ - Μ direction measured at 7 K with 50 eV photons. (c) Symmetrized EDCs of the 𝛼 (7 eV, blue curve), 𝛽 (7 eV, green curve) and δ (50 eV, black curve) bands.  The  red  lines  are  fits  using  phenomenological  model.  Their  superconducting  gap  sizes  are annotated  above.  (d),  (e)  Symmetrized  EDCs  of  the  points  noted  in  the  insets  of  the 𝛼 , 𝛽 pockets, respectively. (f)  Distribution of the in-plane superconducting gap of 𝛼 (upper panel), 𝛽 (lower panel) pockets, respectively. The red and black arrows indicate the Γ - Μ and Γ - Χ directions, respectively. T he error bars reflect the uncertainty in determining the gap sizes.

![Image](https://ac.marcodsn.me/arxiv-markdown-images/2408.00469v1-figure-dff78d23-2752-4e87-b147-81a58475fe4e.jpg)

a

FIG. 3. Kink in the 𝛼 band and its temperature evolution properties. (a) ARPES Spectra measured along the Γ - Μ direction at 7 K, 35 K and 65 K. The presence of a kink in the 𝛼 band is indicated by the black arrow at 7 K. The color bar indicates the photoemission intensity. (b) Corresponding MDCs of the 𝛼 band measured at 7K in panel (a), where peak positions are marked with circles and the kink position is highlighted in blue. (c) The self-energy analysis of the kink reveals anomalies in both Re  (blue circle curve) and Im  (red circle curve) at an energy of approximately 15 meV below the Fermi level. The color bar shows the ARPES spectra intensity. (d) The peak positions of the 𝛼 band, extracted from MDCs at various temperatures. (e) The corresponding electron-boson coupling strength 𝜆𝑒-𝑏 as a function of temperature. The red arrow marks the TC. T he error bars reflect the uncertainty in determining the coupling strength.

![Image](https://ac.marcodsn.me/arxiv-markdown-images/2408.00469v1-figure-85230b4b-e1c9-4f74-86d5-a977dd2ba274.jpg)

Fig 4. Momentum dependent behaviors of the kink in the 𝛼 band. (a), (d) The ARPES spectra measured along the Γ - Χ direction with 𝜃 = 45 ° and the Γ - Μ direction with 𝜃 = 0 ° , respectively. The color bar

![Image](https://ac.marcodsn.me/arxiv-markdown-images/2408.00469v1-figure-c689fbd4-e755-48a1-8a3a-f924f260a9a0.jpg)

indicates the photoemission intensity. (b) ReΣ and ImΣ of the α band for 𝜃 = 45 ° which show negligible anomaly.  (c)  In-plane  dispersions  of  the  band  extracted  from  their  corresponding  MDC  curves presented  at 5 ° intervals  from  the Γ - Μ to  the Γ - Χ directions,  which  are  stacked  with  momentum offsets for a better illustration. (e) The kink energy positions E𝑘𝑖𝑛𝑘 and electron-boson coupling strength 𝜆𝑒-𝑏 , extracted from (c), as a function of 𝜃 angles. They both exhibit suppression upon approaching the Γ - Χ direction. (f) A summary of the E𝑘𝑖𝑛𝑘 (red dots) and the superconducting gap Δ𝛼 (light blue dots) in the 𝛼 band. The kink-corresponding bosonic mode energies are presented as the black dots with a near constant energy of 9 ± 1 meV. T he error bars reflect the uncertainty in determining the gap sizes and coupling strength.
Peng Li Sen Liao Zhicheng Wang Huaxun Li Shiwu Su Jiakang Zhang Ziyuan Chen Zhicheng Jiang Zhengtai Liu Lexian Yang Linwei Huai Junfeng He Shengtao Cui Zhe Sun Yajun Yan Guanghan Cao Dawei Shen Juan Jiang Donglai Feng
Evidence of electron interaction with an unidentified bosonic mode in superconductor CsCa$_2$Fe$_4$As$_4$F$_2$
The kink structure in band dispersion usually refers to a certain
electron-boson interaction, which is crucial in understanding the pairing in
unconventional superconductors. Here we report the evidence of the observation
of a kink structure in Fe-based superconductor CsCa$_2$Fe$_4$As$_4$F$_2$ using
angle-resolved photoemission spectroscopy. The kink shows an orbital selective
and momentum dependent behavior, which is located at 15 meV below Fermi level
along the Gamma-M direction at the band with dxz orbital character and vanishes
when approaching the Gamma-X direction, correlated with a slight decrease of
the superconducting gap. Most importantly, this kink structure disappears when
the superconducting gap closes, indicating that the corresponding bosonic mode
(9 meV) is closely related to superconductivity. However, the origin of this
mode remains unidentified, since it cannot be related to phonons or the spin
resonance mode (15 meV) observed by inelastic neutron scattering. The behavior
of this mode is rather unique and challenges our present understanding of the
superconducting paring mechanism of the bilayer FeAs-based superconductors.